Physica C 299 Ž1998. 59–64 Nonhomogenous transport current density and voltage distribution in isotropic high Tc superconductors V. Bekeris a b a,) , R. Schifini Gladchtein a , M. Monteverde a , P. Dmitruk a , H. Ferrari a , G. Polla b, F. de la Cruz c Facultad de Ciencias Exactas y Naturales, UniÕersidad de Buenos Aires, Ciudad UniÕersitaria, Buenos Aires 1428, Argentina DiÕision del Solido, Departamento de Fısica Comision Buenos Aires 1429, Argentina ´ de Fısica ´ ´ ´ ´ Nacional de Energıa ´ Atomica, ´ c Centro Atomico Bariloche, 8400 San Carlos de Bariloche, Rıo ´ ´ Negro, Argentina Received 7 October 1996; revised 7 October 1997; accepted 9 December 1997 Abstract Transport properties in patterned isotropic high Tc superconducting samples were investigated numerically and experimentally for boundary conditions imposing a nonhomogeneous current flow. Numerical simulations for the voltage distribution were based on a local nonlinear constitutive relation for the current density and the electric field, predicted by the vortex glass model extended to a nonhomogeneous current flow. In experiments the voltage drops at different sample locations were measured as a function of applied current, in a wide temperature range at low magnetic fields, and both the linear and the nonlinear regimes were examined. Our results support a local description, where long-range correlations in the millimeter scale are absent. q 1998 Elsevier Science B.V. PACS: 74.25.Fy; 74.40.q k; 74.80.Bj Keywords: Transport properties; Intergranular vortex phases 1. Introduction Conventional transport properties in sintered, polycrystalline YBa 2 Cu 3 O 7y d ŽYBCO. w1x and La 2y x Sr x CuO4y d ŽLSCO. w2–4x high Tc superconductors are well described within the framework of the vortex glass model w5,6x. There is strong evi- ) Corresponding author. Departamento de Fısica, Pabellon ´ ´ I, Ciudad Universitaria, Buenos Aires 1428, Argentina. Tel.: q5401-782-1007; fax: q54-01-782-7647; e-mail: [email protected] dence that the intergranular vortex system exhibits a second-order phase transition at the field dependent glass temperature, Tg Ž H ., where vortices freeze into a true zero resistance state, showing the scaling behavior predicted for a vortex glass: ErŽ J < t < ÕŽ zy1. . Ž < < 2 Õ ., where E and J are the electric field s Fq y Jr t and the current density, t s < T y Tg <rTg and Õ and z are critical exponents w5,6x. At the phase transition temperature, the E–J characteristics show a power-law behavior. Above Tg Ž H . an ohmic regime at low current density is observed, and below Tg Ž H ., the constitutive relation 0921-4534r98r$19.00 q 1998 Elsevier Science B.V. All rights reserved. PII S 0 9 2 1 - 4 5 3 4 Ž 9 7 . 0 1 8 9 0 - X V. Bekeris et al.r Physica C 299 (1998) 59–64 60 for the electric field and the current density is given by the following expression E ; exp Ž y Ž JcrJ . m . Ž 1. where m is in the range 0–1, and Jc increases as temperature is reduced below the phase transition w5,6x. The length scale for intergranular currents is set by the grain size, d, but at low current densities, the activated vortex loop size L j , becomes larger than d, and the sample appears homogeneous w1x. In the previous works w1–4x where conventional fourterminal transport experiments were performed, the boundary conditions Žsample and current contacts geometry. determine a uniform macroscopic current flow, and the applied current dependence of the voltage drop, V Ž Ia ., can be compared to the EŽ J . characteristics predicted by theory Žsee for example Fig. 3 in Ref. w1x and Fig. 1 in Ref. w3x.. However, future applications may be based on devices constructed with geometries imposing nonhomogeneous transport current densities, not being clear what is the voltage distribution and its current dependence particularly in the highly nonlinear regimes. This possibility has led us to examine multiterminal transport properties in a granular system, where it is possible to separate the influence of anisotropy from the nonhomogeneous current effects arising from the sample geometry. The length scale for the macroscopic current density variation is fixed by the boundary conditions, and we have examined geometries where this length is much larger than the grain size Ž d ; 10 m m., so the homogeneous sample description remains valid. This work is organized as follows: in Section 2 we present a numerical simulation for the current dependence of the bidimensional voltage distribution in the ohmic and the nonlinear regimes, for a sample with the same boundary conditions as one described in experiments. The hypothesis of a scalar apparent resistivity which depends on the total current density is supported by experimental results presented in Section 3. In Section 4 we report results of multiterminal transport measurements in two samples of different geometries; we have measured the voltage drop at several sample locations as a function of applied current in a wide temperature range for low magnetic fields. Conclusions are presented in Section 5. 2. Calculations Our numerical simulation was based on the equation of charge conservation: = P J s 0 and a nonlinear constitutive relation for the local current density J and the electric field E, following Eq. Ž1. with m s 1. This relation is valid only in the vortex-glass phase. Since J s s Ž E ., s s s Ž E . for this nonlinear relation, and E s y= V, the conservation equation expressed in terms of the electric potential V is = P Ž s= V . s 0, which in a 2D case is E Ex EV ž / s Ex E q Ey EV ž / s Ey s 0. Ž 2. To solve numerically this differential equation we apply the finite volume method w7x, using a square grid, to a sample with the geometry shown in the inset of Fig. 1. Note that since s s s Ž E . s s Žy= V ., the discretization equation is nonlinear. We solved this system iterating over the complete grid ŽGauss– Seidel point by point method. until convergence with a relative tolerance of 10y5 is reached. We imposed Neumann boundary conditions at the walls where there is no net current flux Žthat is, EVrEn s 0, where n is the normal direction to the wall. and Dirichlet boundary conditions Ž V s constant. at the current contacts, where there is a net normal current flux entering or leaving the sample. By setting the voltage drop between the current contacts, the cur- Fig. 1. Calculated V12 Žfull line. and V34 Ždotted line. vs. applied current, Ia for the ohmic and the nonlinear regimes. Shown in symbols is V34 Ž s . which stands for g )V34 vs. Ia r f. The inset shows the sample and contacts geometry. V. Bekeris et al.r Physica C 299 (1998) 59–64 rent distributions were calculated and with this the different voltage drops between the voltage contacts. Total applied current, Ia , was calculated integrating the current density. The same procedure was followed for the linear case, where s s s 0 . Fig. 1 shows a log–log plot for V12 Žfull lines. and V34 Ždotted lines. as a function of applied current, for both the linear and nonlinear regimes. Also shown, in symbols, is V34 Ž s . which stands for g )V34 vs. Iarf, where f and g are two scaling factors that map the V34 vs. Ia curve onto the V12 vs. Ia curve in both regimes. For the linear response, it is clear that either a current scaling, Ž Iarh., or a voltage scaling Ž h)V34 . is enough to map V34 onto V12 , where h s f ) g. Nevertheless, for the nonlinear response a unique set of values for f and g is needed in order to map one onto the other. In this particular case we have obtained f s 2.4 and g s 1.3. This is a general result for all the calculated voltage drops, and results from the scaling relation between the local current density and the applied current found in calculations. Therefore f and g depend only on the relative position of contacts Ža change in temperature is represented by a change in s 0 or in Jc , with no 12 influence on f or g ., and will be indicated as f 34 12 and g 34 in what follows. As Vi j –Ia curves can also be mapped onto calculated V–Ia curves for a slab, not shown, they can also be fitted to the expression predicted by the vortex glass model, where the fitted characteristic current density Jc , includes a site-dependent scaling factor. 3. Apparent resistivity A polycrystalline La 1.8 Sr0.2 CuO4yd sample, prepared as described elsewhere w8x, was cut in the shape shown in the inset of Fig. 2 and ground to ; 0.5 mm. The average grain size was 10 m m. Two current and two voltage pairs of gold contacts were sputtered onto the surface of the sample over which silver baking paste was annealed at 6508C for 2 h to improve contact resistance, which resulted below 0.5 V. Two Keithley 224 current sources were used to apply current independently in the x, Ž I x ., and y, Ž I y ., directions. Although the current density is not uniform around the sample corners, it is approximately uniform in the region between voltage contacts. 61 Fig. 2. Ža. R x sVx r I x vs. I x and I y in the low temperature nonlinear regime where R x depends on Ž I x2 q I y2 .1r 2 . The inset shows schematically the sample geometry; Žb. Vx r I x vs. Ž I x2 q I y2 .1r 2 for T s13, 16, 19, 22, 25 and 28 K and Ha s 400 Oe. The voltage drops were measured using a digital scanner and a Keithley 181 nanovoltmeter with approximately 20-nV resolution. Magnetic DC field, Ha , provided by a superconducting solenoid, was applied perpendicular to the sample in the normal state, and the sample was field cooled to several temperatures. Vx and Vy were measured as a function of increasing I x for different I y . Because of symmetry we refer only to the Vx results. I y generated no voltage drop in the x direction ŽHall effects are negligible w9x., and R x was evaluated as VxrI x after proper current inversion to make negligible spurious thermal e.f.m. effects. Fig. 2Ža. shows R x Ž I x , I y . for T s 19 K and Ha s 400 Oe, and in Fig. 2Žb. we plot R x vs. Ž I x2 q I y2 .1r2 for T s 13, 16, 19, 22, 25 and 28 K and Ha s 400 Oe. It is clear that R x is a function of the absolute value of the total applied current. Similar results were obtained for Ha s 0 and 100 Oe, supporting a total current density dependence of the resistivity. 62 V. Bekeris et al.r Physica C 299 (1998) 59–64 4. Multiterminal I–V characteristics For the experimental study of the voltage distribution, two polycrystalline La 1.8 Sr0.2 CuO4yd samples w8x from different batches were cut in the shapes shown in Fig. 3 and ground to ; 0.5 mm Žsample A. and ; 0.7 mm Žsample B.. Two low-resistance wide-current contacts and six 0.2-mm-diameter voltage contacts, made following the procedure described in Section 3, are shown schematically in the figure for sample A. Sample B was provided with two pairs of voltage contacts. In the ohmic regime the superconducting transition voltage drop was measured across several contact pairs for Ha s 0 and Ia s 500 m A. Fig. 4 shows in full lines V12 , V34 and V56 as a function of temperature for sample A. Contacts 12 were arbitrarily chosen as reference, and shown in symbols is Ž ij standing for 34 and 56., where h12 i j )Vi j vs. T 12 h12 s 2.4 and h 34 56 s 10.7 are the voltage scaling constants, indicating that the average current density, - Ji j ) is lower than - J12 ) . As expected for a linear regime, h12 i j is temperature independent up to 300 K Žnot shown in the figure.. Similar results were obtained for the resistive transition of sample B, with h12 34 s 5.8. We present next the multiterminal I–V characteristics for sample A at Ha s 400 Oe. We show in Fig. 5 the log–log plot of: Ža. V12 vs. Ia ; Žb. V34 vs. Ia and Žc. V56 vs. Ia for temperatures between 14 and 27 K. For every temperature, voltage is first detected between contact pair 12, and current has to be further increased so that dissipation across the next pair of voltage contacts exceeds voltage resolution. The collection of curves at each location was mapped onto the collection of V12 vs. Ia curves, as Fig. 3. Layout of the geometry, current and voltage contacts for Ža. sample A; Žb. sample B. Lengths are given in mm. Fig. 4. Vi j vs. temperature for Ia s 500 m A and Ha s 0 for sample A, where ijs12, 34, 56 Žsolid.. Also shown is h12 34 )V34 12 12 Žv ., and h12 Ž . 56 )V56 I , where h 34 s 2.4 and h 56 s10.7. Fig. 5. Ža. V12 vs. Ia ; Žb. V34 vs. Ia and Žc. V56 vs. Ia . In all cases, T s14, 15, 16, 17, 19, 21, 23, 25 and 27 K, with Ha s 400 Oe for sample A. V. Bekeris et al.r Physica C 299 (1998) 59–64 63 Table 2 Geometrical scaling constants f i12j and g i12j for different contact pairs ij for sample B Scaling factor f g Contacts 34 13 24 4.2 1.4 0.5 5.0 1.0 2.2 Applied current must be divided by f i12j and voltage must be multiplied by g i12j to map each curve onto V12 Ž Ia .. Fig. 6. Ža. V12 vs. Ia Žsolid line. and Vi j Ž s ., which stands for Žsymbols., at T s14, 15, 16, 17, 19, 21, 23, g i12j )Vi j vs. Ia r f i12 j 25 and 27 K, with Ha s 400 Oe for sample A. Žb. V vs. Ia Žsolid line. for a strip of the same batch as sample B. Also shown is g )V12 vs. Ia r f Žin symbols. for sample B, Ha s 0. shown in Fig. 6Ža.. Table 1 shows the site dependent scaling factors. The product f i12j ) g i12j s h12 i j , where Ž . h12 i j is the ohmic scaling factor see Fig. 4 . Similar results were obtained for sample B at 20, 40, 60 and Table 1 Geometrical scaling constants f i12j and g i12j for different contact pairs ij for sample A Scaling factor f g Contacts 34 56 24 46 26 2 1.3 3.5 3.1 0.7 4.1 1.5 3.4 0.9 2.2 Applied current must be divided by f i12j and voltage must be multiplied by g i12j to map each curve onto V12 Ž Ia .. 80 Oe, and the field independent scaling factors are presented in Table 2. In Fig. 6Žb. we show V–Ia characteristics for a strip 7 = 2 = 0.7 mm3 of the same batch as sample B Žfull lines. at Ha s 0 and different temperatures, which can be described within the vortex-glass model w2–4x. Also shown Žsymbols. is 0.88)V12 vs. Iar1.7 for sample B. If we fit the data V vs. Ia Žslab. and V12 vs. Ia Žsample B. to the expression V s V0 expŽyŽ IcrIa . m ., for T s 28 K, we obtain for the slab a characteristic current Ic Žslab. approximately equal to Ž1r2. = Ic ŽSample B.. The mapping procedure provides a comparative description that is useful to avoid fitting every measured curve. It is well established w10x that the low current-density regime at T ) Tg Ž H ., crosses over to a nonlinear regime for J ) Jcr , but it was not observed in the present work due to our voltage resolution. Nevertheless, the result f i12j ) g i12j s h12 i j is an indication that the scaling procedure will map the complete curves. 5. Conclusions We have studied the transport properties in isotropic LSCO high-Tc superconducting samples which were patterned to force a nonhomogeneous transport current flow, and were provided with several voltage contact pairs, ij, to measure the applied current dependence of the voltage distribution. We have found that the Vi j –Ia characteristics map onto conventional homogeneous current flow V–Ia characteristics, and therefore follow the predictions of the vortex glass model, with scaled relevant parameters. Numerical simulations based on a constitutive relation for the current density and the electric field predicted for the vortex glass phase and for the ohmic regime, also exhibit mapping properties arising from the proportionality between applied current 64 V. Bekeris et al.r Physica C 299 (1998) 59–64 and local current density found in calculations. Our present results support a local electrodynamical description and the absence of long-range correlations in the intergranular vortex motion in the mm length scale. Future measurements in patterned films, where the voltage contact distances may be reduced below the millimeter scale will be performed. Acknowledgements We thank G. Gnavi and A. Lopez Davalos for ´ ´ fruitful discussions. We acknowledge E. Rodriguez for careful reading of the manuscript. This work was partially supported by CONICET PID 303320088 and UBA EX018 grants. References w1x T.K. Worthington, E. Olson, C.S. Nichols, T.M. Shaw, D.R. Clarke, Phys. Rev. B 43 Ž1991. 10538. w2x R. Decca, PhD Thesis, Instituto Balseiro, Universidad Nacional de Cuyo, Argentina, 1994. w3x R. Decca, Physica C 235–240 Ž1994. 1639. w4x L. Urba, C. Acha, V. Bekeris, Physica C 279 Ž1997. 95. w5x M.P.A. Fisher, Phys. Rev. Lett. 62 Ž1989. 1415. w6x D.S. Fisher, M.P.A. Fisher, D.A. Huse, Phys. Rev. B 43 Ž1991. 130. w7x S.V. Patankar, Numerical Heat Transfer and Fluid Flow, Hemisphere Publishing, Mc Graw-Hill, New York, 1981. w8x R. Crubellati, P. Smichowski, D. Batistoni, G. Polla, E. Manghi, Solid State Commun. 75 Ž1990. 101. w9x M. Petravic, A. Hamzic, B. Leontic, L. Forro, Int. J. Mod. Phys. B 1 Ž34. Ž1987. 1067. w10x G. Blatter, M.V. Feigelman, V.B. Geshkenbein, A.I. Larkin, M.V. Vinokur, Rev. Mod. Phys. 66 Ž1994. 1125.